| ||Format||Pages||Price|| |
|PDF Version||4||$37.00||  ADD TO CART|
|Print Version||4||$37.00||  ADD TO CART|
Significance and Use
4.1 This test method is useful in that the joint configuration closely simulates the actual joint configuration of many bonded assemblies. Surface preparation of the adherends can affect the apparent shear strength of the adhesive and can be one of the variables under study.
4.2 This test method is also useful as an in-process quality control test for laminated assemblies. In practice the laminated assembly is either made over size and test specimens removed from it or a percentage of the assemblies are destructively tested.
4.3 The misuse of strength values obtained from this test method as design allowable stress values for structural joints could lead to product failure, property damage, and human injury. The apparent shear strength of an adhesive obtained from a given small single-lap specimen may differ from that obtained from a joint made with different adherends or by a different bonding process. The normal variation of temperature and moisture in the service environment causes the adherends and the adhesive to swell and shrink. The adherends and adhesive are likely to have different thermal and moisture coefficients of expansion.
4.3.1 Even in small specimens, short-term environmental changes can induce internal stresses or chemical changes in the adhesive that permanently affect the apparent strength and other mechanical properties of the adhesive. The problem of predicting joint behavior in a changing environment is even more difficult if a different type of adherend is used in a larger structural joint than was used in the small specimen.
4.4 The apparent shear strength measured with a single-lap specimen is not suitable for determining design allowable stresses for designing structural joints that differ in any manner from the joints tested without thorough analysis and understanding of the joint and adhesive behaviors.
4.5 Single-lap tests may be used for comparing and selecting adhesives or bonding processes for susceptibility to fatigue and environmental changes, but such comparisons must be made with great caution since different adhesives may respond differently in different joints. Review Guide D4896 for further discussion of concepts for interpretation of adhesive-bonded single-lap joint data.
1.1 This test method (Note 1) is intended for determining the comparative shear strengths of adhesives in large area joints when tested on a standard single-lap-joint specimen and under specified conditions of preparation and testing. Adhesives respond differently in small versus large area joints (Note 2).
1.2 The values stated in SI units are to be regarded as the standard. The values given in parentheses are for information only.
1.3 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
A167 Specification for Stainless and Heat-Resisting Chromium-Nickel Steel Plate, Sheet, and Strip
A366/A366M Specification for Commercial Steel (CS) Sheet, Carbon, (0.15 Maximum Percent) Cold-Rolled
B36/B36M Specification for Brass Plate, Sheet, Strip, And Rolled Bar
B152/B152M Specification for Copper Sheet, Strip, Plate, and Rolled Bar
B209 Specification for Aluminum and Aluminum-Alloy Sheet and Plate
B265 Specification for Titanium and Titanium Alloy Strip, Sheet, and Plate
D907 Terminology of Adhesives
D2093 Practice for Preparation of Surfaces of Plastics Prior to Adhesive Bonding
D2651 Guide for Preparation of Metal Surfaces for Adhesive Bonding
D3933 Guide for Preparation of Aluminum Surfaces for Structural Adhesives Bonding (Phosphoric Acid Anodizing)
D4896 Guide for Use of Adhesive-Bonded Single Lap-Joint Specimen Test Results
E4 Practices for Force Verification of Testing Machines
ICS Number Code 83.180 (Adhesives)
UNSPSC Code 41113046(Adhesion tester); 31201601(Chemical adhesives)